Elucidation of Softening Mechanism in Rinse-Cycle Fabric Softeners. Part 2: Uneven Adsorption—The Key Phenomenon to the Effect of Fabric Softeners
- First Online:
We investigated the actual factor determining the softening effect of a fabric softener. The adsorption area of the softener on model cotton cloths and yarns was identified using bromophenol blue. There was almost no softener at the cross-points of the yarns in the cloth samples or in the inner part of the yarns. The softening performance was better when there was less softener at the cross-points of the yarns than when the yarns were evenly covered by the softener. Thus we conclude that the presence of softener at the cross-points of yarns is not a vital factor in the softening effect. In addition, more softener was found on the outer part of the yarn than the inner part, indicating gradation in the adsorption pattern of the softener. Thus, we propose that more softener is adsorbed on the exposed part of the yarn in a cloth, and the formation of a hydrogen-bonding network containing bound water is inhibited, thus softening the outer part of the yarn. However, the presence of a small amount of softener in the inner part of the yarn preserves the hydrogen-bonding network. Favorable elasticity, or bounce, of the yarns and cloth is realized when an appropriate amount of softener is used. Excess softener would reach the inner part of the yarn, reducing the diameter of the core part of the yarn, making the cloth appear wilted.
KeywordsFabric softener Mechanism Cotton Bound water Hydrogen bonding Cross-linking Gradation Bromophenol-blue coloration method
There has been much discussion on the mechanism of adsorption of softeners on cotton fibers. The most widely accepted explanation is that the cationically charged vesicles of the softener are adsorbed on the surface of the anionically charged cotton fibers [3, 4]. However, there is uncertainty associated with this mechanism, because the sequence of adsorption is thermodynamically unfavorable: adsorption is followed by the formation of multilayers between the fibers and water by the cationic surfactants, which are sparingly soluble in water, together with subsequent formation of a monolayer between the fibers and air. Crutzen  suggested that hydrophobic interactions derived from the long alkyl chains of cationic surfactants are an important driving force in adsorption, because the softener can be adsorbed even on uncharged fiber surfaces. Minegishi  reported that the time required to attain adsorption equilibrium is strongly influenced by a mechanical force when the softener is adsorbed on cotton fibers. This finding also indicates that the dominant factor is not electrostatic interactions, but the “collision” between the fibers and vesicles of the softener. Okumura  reported that fabric softener adsorbed on the surface of cotton maintains uniform multilayered states. Nakamura et al.  reported that the softener exists as an “interdigitated structure” after the collapse of vesicles during drying. Sakai et al.  recently used atomic force microscopy to observe the adsorption on the surface of mica, and reported that the vesicles adsorbed by collision immediately expanded to form a double-layered molecular membrane. The adsorption state of the softener molecules was then maintained without loss of the molecules from the surface, because of the electrostatic interaction between the anionic part of the cotton surface and the cationic moiety of the softener molecule.
In this study, we aimed to deepen our understanding of the adsorption behavior of a fabric softener by using a cationic surfactant indicator to focus on the assembled cotton fibers (yarn and cloth). We also considered the reason for the softening effect based on our findings, some of which were reported in our previous papers [1, 2], while others are presented here for the first time. The results show that the existence of the softener at the cross-points of the yarns in the cloth has no direct role in the “softness” of the cloth, leading us to conclude that reduced friction or lubrication at the cross-points is not the main reason for the softness caused by fabric softeners.
Thick Cotton Yarn
Cotton knitting yarns (diameter: 2.7 mm; Amiami Cotton, manufactured by Hamanaka Corp., Japan) were used as samples for the adsorption experiments. Before the experiments, 18 g of the yarns was thoroughly pre-washed with 1000 mL of a solvent [CHCl3/MeOH = 1/1 (wt. ratio)] and stirred for 5 min. This pre-washing process was carried out three times to remove the pre-treatment oils adsorbed on the yarn during the yarn-making process.
Model Cotton Cloths
Details of towel samples
Twist of Pile yarn (turns/m)b
Ground warp (tex)
Pile warp (tex)
Distearyl dimethyl ammonium chloride (DODAC; Tokyo Kasei Corp., Japan) and Esteramide (EA; Kao Corp., Japan) were used without purification as the model softeners. The concentration of softener used for treatment of the yarns and cloths was chosen according to the testing conditions described in the following softener-treatment experiments.
Softener Treatment for Thick Cotton Yarn
Ion-exchanged water (400 mL) and a 0.5 % softener dispersion (0.8 mL) were placed in a 500-mL beaker and stirred for 1 min. The pre-washed thick cotton yarns (4 g) were immersed in this aqueous solution and stirred for 48 min (the bath ratio was set to 100). The treated wet yarns were spread on a sheet of polypropylene (PP; PC-8186, Sekisui Chemical Co.,Ltd., Japan) and allowed to dry naturally.
Softener Treatment for Model Cotton Cloths
Ion-exchanged water (400 mL) and a 0.5 % softener dispersion (0.8 mL) were placed in a 500-mL beaker and stirred for 1 min. Three pieces of the woven model cotton cloths were immersed in this aqueous solution and stirred for 5 min (the bath ratio was 100). The treated wet cloths were spread on the PP sheet and allowed to dry naturally.
Softener Treatment for Cotton Towels
Two pre-washed cotton towels (78 g each) were treated with an aqueous solution of the softener in a small washing machine (MiniMini Washer NA-35, Panasonic Corp., Japan). The bath ratio was set to 30, and 47 L of tap water (Wakayama city, Japan) was used at 25 °C. First, the softener [0–0.3 % on the weight of fabric (o.w.f.)] was dispersed in the water with sufficient stirring; then, two towels were immersed in the water and stirred for 5 min. Preliminary studies [1, 2] showed that the rate of softener adsorption on the fibers of these towels reached nearly 100 % within 5 min. Following treatment with the softener, the towels were spin-dried in a two-tank washing machine (PS-H35L, Hitachi Corp., Japan) for 3 min and manually fluffed five times. Samples from the pile area of the towels were used to measure the shear, friction, compression, and tensile properties.
Measurement of Amount of Adsorbed Softener
Extraction of Softener Adsorbed on Yarns
Methanol (80 g, high-performance liquid chromatography [HPLC] grade; Wako Pure Chemical Industries, Ltd., Japan) and HCl (0.8 g, 35 % aqueous solution; Wako Pure Chemical Industries, Ltd., Japan) were poured into a 100-mL glass container. The thick cotton yarns (around 1.0 g) that had been pre-washed, treated with the softener, and dried were then added and subjected to ultrasonic agitation for 20 min. The resulting liquid was diluted with methanol, as required, until it reached 1/100th to 1/1000th of its original concentration. The amount of softener adsorbed on the yarns was measured three times by HPLC-mass spectrometry (HPLC–MS).
Equipment and Measurement Conditions
The amount of softener adsorbed on the cloths and yarns for this study was measured by an HPLC–MS (Prominence UFLC; Shimazu Seisakusho, Japan) system and an MS system (LCMS-2010; Shimazu Seisakusho, Japan) with electrospray ionization (ESI) in positive mode. The ionization conditions for electrospraying were optimized by the automatic calibration system. The analytical column, Unison UK-C18 HT (diameter 2 mm × length 50 mm, diameter of gel particles: 3 μm; Imtakt, Japan), was operated at 40 °C. A 10-mM aqueous acetic ammonium solution was used as mobile phase A, and a 10-mM acetic ammonium MeOH solution was used as mobile phase B. A gradient was set from 50 to 100 % B over 2 min and maintained for 3 min at a flow rate of 0.5 mL/min. For selected ion monitoring (SIM) measurements, the MS ionization mode was set as positive, and protonated molecular ions, [M+H]+, were used: mass to charge ratio, m/z = 550.7 for DODAC in the SIM mode.
Observation of the Adsorption State of the Fabric Softener
Evaluation of Color Intensity by the BPB Method
Shear Property Measurements by the KES (Kawabata Evaluation System) Method
The shear properties of each sample were measured using the Kawabata evaluation system (KES). An automatic shear tester (KES-FB-1-AUTO-A; Katotech Corp., Japan) was employed, and samples were sheared under a load of 10 gf/cm2 at a shear rate of 0.417 mm/s. The hysteresis of shear force (2HG, measured in gf/cm) at a shear angle of 0.5° was obtained during the dynamic process at 25 °C and 50 % RH. As the value of 2HG became higher, the sample showed less resilience. The measurements were carried out six times.
Frictional Property Measurements by the KES Method
An automatic frictional tester (KES-FB-4-AUTO-A; Katotech Corp., Japan) was employed to carry out frictional property measurements on each sample. During the measurement, 20 gf/cm of tension was added, and the contact device made of piano wire (the weight of the load was approximately 50 gf) was moved over a length of 2.5 cm at a speed of 1 mm/s on the pile. In doing so, the average mean coefficient of friction (MIU) was measured at 25 °C and 50 % RH. The measurements were carried out six times.
Compression Property Measurements by the KES Method
An automatic compression tester (KES-FB-3-AUTO-A, Katotech Corp., Japan) was employed to measure the compression properties of each sample. The samples were compressed under a maximum force of 50 gf/cm2 at a compression speed of 0.02 mm/s. The work of compression (WC, gf/cm) was measured during the dynamic process at 25 °C and 50 % RH. As WC increased, it became easier to compress the sample. The measurements were carried out six times.
Tensile Property Measurements by the KES Method
An automatic tensile tester (KES-FB-1-AUTO-A; Katotech Corp. Japan) was employed to carry out tensile property measurements on each sample. The samples were measured under the maximum load of 500 gf/cm2 at a tensile rate of 0.2 mm/s. The tensile energy (WT, gf/cm) was measured during the dynamic process at 25 °C and 50 % RH. As WT increased, it became easier to stretch the sample. The measurements were carried out six times.
Evaluation of Yarn Pull-Out Force from a Plain-Woven Cloth
One piece of yarn from a 7 cm × 3 cm area of the plain-woven cloth was cut from the middle position, up to 2 cm from the bottom of the cloth, and pulled out from the cloth. The pull-out force was measured using Sebastian’s method  at a speed of 1 cm/min with a universal testing machine (TENSILON, A&D, Japan).
Adsorption State of the Softener
Staining tests using a 4 % aqueous osmium tetroxide solution were carried out both for the softener on a glass plate and on the model yarns (100-fold concentration; 10 % o.w.f.). Effective staining of the yarn was visually confirmed. The softener-treated model yarn was steam-stained with a 4 % aqueous osmium tetroxide solution and embedded in a visible-light-curable resin (D-800, JEOL, Japan). A smooth cross section was then prepared using a microtome (Leica, Germany) for further analysis. Field-emission scanning electron microscopy (FE-SEM; JSM-7600F, JEOL, Japan) observations (10 kV), energy-dispersive X-ray spectrometry (EDS; INCA Energy, Oxford Instruments, UK) analysis (10 kV), and time-of-flight secondary ion mass spectrometry (TOF–SIMS; TOF–SIMS IV, IONTOF, Germany) analysis (25 kV) were performed. SEM observation using a backscattered electron detector showed good contrast corresponding to the element number. In terms of both sensitivity and resolution, the TOF–SIMS results gave the best overview of the distribution of softener molecules in the cross section.
Evaluation of Softening Effect Using Model Cloths
The level of softness of the model cloths was evaluated via sensory tests performed by five expert panelists. The evaluation was carried out by compression of the cloth between the panelists’ palms.
Evaluation of Softening Effect Using Towels
Softener EA (Esteramide, Kao Corp., Japan) was used for preparing reference towels to determine the level of softness of the tested towels. The concentrations of EA were set to six grades: 0, 0.025, 0.05, 0.075, 0.1, and 0.125 % o.w.f. (the softening levels corresponding to each grade were denoted on a scale of 1 to 6). The level of softness was evaluated by five panelists through comparison sensory tests using the reference towels.
Results and Discussion
BPB Coloring Method for Determining the Softener Adsorption Area
First, 1 mL of 0.5 wt % aqueous softener dispersion was released in drops onto the central part of a plain woven cloth (5 cm × 5 cm). The dispersion area was then marked using a permanent marker, and the cloth was allowed to dry naturally. The cloth was then washed in 3 L of ion-exchanged water, followed by immersion in the BPB coloring reagent. BPB is known to be a good indicator of cationic surfactants, and we were able to visually identify the area in which the softener was adsorbed. The resulting blue-stained areas indicated the presence of the softener. We found that the softener did not wash off or drift from its original position after the sample was cleaned with ion-exchanged water. Thus this coloring method is useful for identifying areas on a sample where the softener exists.
Role of the Yarn Cross-Points in the Cloth in Relation to the Softening Effect
Postulate #1: The Softener at the Cross-Point of a Cloth Did Not Play an Influential Role in Overall Softening
To accurately compare the two samples, the amount of adsorbed softener must be set to the same level. When sample (a) was prepared, we stirred for 5 min to allow the softener to be adsorbed on the cotton surface. This is the same condition as that used to prepare the model cotton towels. When the HPLC–MS was used, the resultant amount of adsorbed softener was 762 mg/kg (corresponding to an adsorption rate of 76.2 %). However, when sample (b) was prepared, the amount of adsorbed softener was as low as 369 mg/kg (the adsorption rate was 36.9 %), despite stirring the sample for the same amount of time. To overcome this imbalance, the yarn treatment time was increased to 48 min, at which point the amount of softener adsorbed by sample (a) was 800 mg/kg. The significant difference between the adsorption rates of these two samples might have been caused by the difference in the frequency of collisions between vesicles and fibers. This collision frequency was lower in the yarns because they drifted more easily, synchronizing with the flow of the aqueous softener solution.
Based on the above results, we can interpret the mechanism of softener vesicle adsorption on fibers as “adhesion by collision,” which supports the findings of Minegishi  and Sakai et al. . In this mechanism, the softener has a tendency to be adsorbed on the exposed parts of the fibers or cloth sample, because the adsorption is controlled mainly by the collision of the softener vesicles with the fibers.
We then tried to compare the softening effect by performing sensory tests (n = 3) using samples (a) and (b) (Fig. 6). Before the tests, we confirmed that there was no difference between the two samples when no softener was used.
As mentioned before, sample (a) showed uneven adsorption of the softener. In other words, the blue coloration indicating the existence of softener molecules, i.e., cationic agents, was less prevalent at the cross-points in the yarns of sample (a). The fact that sample (a) showed higher softening clearly demonstrates that the adsorption of a softener at the cross-points in a cloth has no significant impact; however, adsorption on the exposed part of the cloth is important for effective softening. The reproducibility of this phenomenon was confirmed using model cotton cloths of different densities (loosely woven and tightly woven samples) (Fig. 2).
Postulate #2: The Softener at the Cross-Point of a Cloth Played an Influential Role in Overall Softening
The KES method for evaluating the shearing, surface, compressional, and tensile properties was applied to towels prepared by treatment with the softener at different concentrations (0–0.2 % o.w.f.).
Interpretation of the Role of Cross-Points
The two results described under Postulates #1 and #2 lead to contradictory conclusions, i.e., “cross-points are not influential” versus “cross-points are influential” in the softening of a piece of cloth. Therefore, we examined the pull-out force measurement process more carefully, and an interesting fact was revealed. The point corresponding to the maximum pull-out force in the plain woven cloth sample was not located at the position immediately after the starting point of the pull-out process, but 14 mm away from the starting position, as shown in Fig. 10a (left panel), when the actual sample size was only 50 mm (Fig. 10a, right panel; the total size of the sample was 70 mm). This large shift, i.e., 14 mm, is quite aberrant if we compare it with pull-out measurement results commonly observed in other studies. When softeners of different concentrations were used (Fig. 10a), the same type of unusual shift was observed.
If we consider only the effect of static and kinetic friction between yarns or fibers because the number of cross-points in a cloth sample is the greatest at the very early stage of the pull-out action, the frictional force must have the greatest influence in this early stage. However, it should decrease gradually in the latter stages, such that the force curve should be similar to that shown in Fig. 10b, in which a peak appears in the very early stage. What we found in our experiment (Fig. 10a, left panel), however, was quite different.
To clarify the reason for the two contradictory theories about the role of cross-points, a hypothesis was developed and examined, as described below.
When no softener is used, full adhesion occurs by hydrogen bonding between the yarns or fibers [1, 2]. In the pull-out force measurement process, when one yarn is selected and pulled upward, deformation of the cloth structure occurs because this yarn is adhered to the horizontal yarns in the cloth sample until the hydrogen bonds begin to break. As a result, the peak of the pull-out force curve shifts to the right, as seen in the left panel of Fig. 10a. When a softener is used, the pull-out force decreases, but the shape of the force curve remains the same, and the shift of the peak to the right still occurs because some adhesion always remains.
When examining the shear, it is important to remember that hydrogen bonding and its breakage near the cross-points of the yarns is controlled by the presence of softener in the same manner as that shown in the pull-out force measurement results. However, we found that the softness was unrelated to the cross-points, as discussed under Postulate #1 and shown in Figs. 6 and 7. Thus the shear hysteresis or pull-out force is considered to be “indirectly” correlated with the softness, owing to the interposition of the hydrogen bonding network between the fibers or yarns.
In order to verify the above hypothesis, we tried to quantitatively evaluate the change in the degree of coloration in a strand of yarn from a model cotton cloth. The degree of permeation of the softener from the S and U directions was measured, as shown in Fig. 12.
Observation of the Cross Section of a Model Strand of Yarn
We successfully stained a cross section of a strand of yarn treated with the softener with osmium tetroxide, and the yarn was partially blackened. Because the blackening was very weak for the untreated yarn, staining was found to be selective for the softener. Using osmium tetroxide staining, detailed SEM–EDS analysis of a single fiber was possible, but overall analysis at the yarn level with suitable sensitivity was difficult.
Amount of Adsorbed Softener in the Inner and Outer Parts of a Thick Strand of Yarn
Given such results, the softener was surely considered to be more concentrated on the surface or outer part of yarns than in the inner part. Moreover, the above-mentioned “gradation” actually existed.
Relationship Between the Softener Concentration and Softening Effect
Mechanism of the Softening Effect by Softeners
Based on the information hitherto described, a new mechanistic concept of the softening effect is proposed by considering that the cloth or yarns, or both, are an assembled architecture composed of fibers. As mentioned in Postulate #1, the amount of adsorbed softener was lower at the cross-point and in the inner part of the yarn. The softener was thus considered to have a tendency to be adsorbed on the exposed part of the fiber assembly.
This result shows that the softening effect of a softener is not caused mainly by lubrication at the cross-points of a cloth or between yarns. When we focused on one strand of yarn as an assembly consisting of single fibers, there was a difference between the amount of adsorbed softener in the inner and outer parts, i.e., gradation was observed.
A good balance of both of these states is important for realizing the proper bouncy feel. Using a rough model in which a strand of yarn is imagined as a cylinder, as shown in Fig. 18, all parts of the yarn are hardened by the cross-linking of the hydrogen-bonding network when no softener is used. When a proper amount of softener is used, a good balance of a soft and fluffy outside and a hard inner side are realized, resulting in the bouncy feel. Furthermore, when an excess amount of softener is used, it diffuses into the inner part of the yarn, reducing the diameter of the cylinder. Because the rigidity of the cylinder is proportional to the fourth power of the diameter, the slight difference in the diameter causes a significant difference in the rigidity. Moreover, when the yarn is treated with an excess amount of softener, the core diameter decreases, the bouncy feel is not obtained, and the yarn wilts.
Softener adhesion to the cotton fiber assembly in the cloth and yarn was observed using the coloration method. The softener concentration was found to be very low at the cross-points of the cloth and high in the exposed part of the fiber assemblies. These results coincide with the mechanisms reported by Minegishi  and Sakai et al. , according to which the softener is considered to be adsorbed on the fiber surface because of collisions and subsequent adhesion of the vesicles.
When we investigated the softness of the model cloth in which the softener was present mainly on the exposed part and rarely at the cross-points (unevenly treated cloth), this cloth was found to be softer than the cloth in which softener was evenly adsorbed. The cloth containing less softener at the cross-points was apparently softer, contrary to the “lubrication-based” expectation. In other words, these results support the idea that increased sliding at the cross-points using softener is not necessary, even if the lubrication theory is considered to hold true based on the results of shear force and yarn pull-out force measurements. Furthermore, when we investigated the amount of softener adsorbed in the inner and outer parts of the yarn, the concentration in the outer part was higher, and there was a concentration gradient from the outer to the inner side. Thus, the softener was easily adsorbed on the exposed part of the yarn.
Based on these results and our preliminary studies [1, 2], we propose the following new softening mechanism for fabric softeners. First, the formation of the hydrogen-bonding network by bound water between cotton fibers is effectively inhibited by the preferential adsorption of softener at the outer part of yarns or cloths. In contrast, softener adsorption in the inner part of a strand of yarn is lower and the structure is harder because of the hydrogen bonding. Thus, the appropriate hardness is maintained in the inner part. Because of the good balance of these two phenomena, the favorable bouncy feel for the cloth or yarns is realized. When an excess amount of softener is used, however, the softener that is originally adhered to the exposed surface of the strand gradually penetrates the inner part of the strand, decreasing the hydrogen bonding, which in turn results in a reduction in the hardness and bouncy feel. This penetration inside the yarn is considered to be the cause of the wilted feel of a cloth with excess softener.
We would like to offer our deepest gratitude to Mr. Shigeru Tamura, Vice President of Global R&D for Household Products Research at Kao Corporation, Japan. We also thank Prof. Kaoru Tsujii of Hokkaido University and Prof. Masayuki Takatera of Shinshu University for their constructive comments and warm encouragement.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.